Strain-Rate Sensitive Behavior of Cement Paste and iri/projects/concrete/HSD.pdf Strain-Rate...
Embed Size (px)
Transcript of Strain-Rate Sensitive Behavior of Cement Paste and iri/projects/concrete/HSD.pdf Strain-Rate...
ACI MATERIALS JOURNAL TECHNICAL PAPER Title no. 87-M55
Strain-Rate Sensitive Behavior of Cement Paste and Mortar in Compression.
by Shraddhakar Harsh, Zhenjia Shen, and David Darwin
The strain-rate sensitivity of the cement paste and mortar constitu-ents of concrete is studied experimentally. Saturated cement paste and mortar specimens are loaded in compression to 15,000 microstrains, 27 to 29 days after casting, using strain rates ranging from 0.3 to 300,000 microstrainslsec. Water-cement ratios of 0.3, 0.4, and 0.5 are used. Strain-rate sensitivity of the materials is measured in terms of the initial elastic moduli, maximum stress, and corresponding strain. The initial elastic moduli and the strength of cement paste and mor-tar increase by 7 percent and 15 percent, respectively, with each or-der of magnitude increase in strain rate. The strain at the maximum stress is the greatest for the lowest strain rate. With an increase in strain rate, the strain at the maximum stress first decreases and then increases.
Keywords: cement pastes; compression; compressive strength; concretes; mod ulus of elasticity; mortars (material); Poisson ratio; sands; saturation; strains; stresses; stress-strain diagram.
The strain-rate sensitive behavior of concrete and its constituents has been under investigation for several decades.1 The rate sensitivity has generally been meas-ured in terms of the strength, modulus of elasticity, or the strain at the maximum stress in compression. It has also been measured in terms of Poisson's ratio, tensile strength, or flexural strength.
In most studies, the compressive strength of concrete and its constituents has been observed to increase ap-proximately linearly with each order of magnitude (factor of 10) increase in strain rate, up to moderate strain rates, e.g., about 1000 microstrains/sec. Gener-ally, the increase has been 7 to 15 percent with each or-der of magnitude increase in strain rate or stress rate. 1-s In a few cases, however, the increase has been consid-erably less910 or insignificant. 211 At higher than moder-ate strain rates (i.e., above 1000 microstrains/sec), there has been less agreement among various studies. Some have observed that the linear relation is maintained up to strain rates as high as 8 x 108 microstrains/sec, 12 while others have found the relation to be either con-cave upward, 1013 15 or concave downward1617 with in-creasing strain rate.
The modulus of elasticity, while less sensitive than strength, 1119 has also been found to increase with strain rate.
The effect of strain rate on the Poisson's ratio of on-crete has not been investigated extensively. 220 No re-sults are available on the strain-rate sensitivity of Pois-son's ratio for cement paste and mortar.
There is little agreement among researchers on the rate-sensitive behavior of the strain at the maximum stress. Some have found it to increase, 102021 while oth-ers have found it to remain almost constant1922 or even decrease21723 with increasing strain rate. Generally, in cases when it was found to increase, the tests were done at higher strain rates.
In spite of the considerable number of studies on the rate sensitivity of concrete and its constituents, there are significant disagreements. The disagreements can sometimes be attributed to changes in test conditions, such as the moisture content of specimens, the curing conditions, or the range of strain rates used. For ex-ample, the insignificant increase in compressive strength with increasing strain rate observed by Dhir and Sangha2 was most likely due to the low moisture con-tent of their specimens, caused by storage in air for 10 weeks.
The purpose of this study is to help improve the knowledge of concrete by studying the rate-sensitive re-sponse of its constituents, cement paste, and mortar. The study is aimed at gathering basic information on the response of fully saturated materials, that is, materials that are not affected by drying. A study of materials in the saturated state, while not universally applicable to all concrete, directly applies to a large percentage of concrete structures, which remain satu-rated at depth. Compressive stress-strain response is measured in terms of the peak stress ,fp, the strain cor-responding to the peak stress Ep, the initial modulus of
AC! Materials Journal, V. 87, No. 5, September-October 1990. Received June 23, 1989, and reviewed under Institute publication policies.
Copyright 1990, American Concrete Institute. All rights reserved, includiing the making of copies unless permission is obtained from the copyright propri-etors. Pertinent discussion will be published in the July-AugusM991 AC! Ma-terials Journal if received by Apr. I, 1991.
ACI Materials Journal I September-October 1990
ACI member Shraddhakar Harsh is a design engineer with McGraw Construc-tion, Ashland, Kentucky. He holds a BS from Brita Institute of Technology and Science, Pilani, India, an MBA from Podar Institute of Management, Jaipur, India, and MS and PhD degrees from the University of Kansas. He has seven years of experience in the construction industry.
Zhmjia Shen is a visiting scholar at the University of Manitoba. He recently completed three years of study at the University of Kansas. He holds a master of science degree from Tongji University, Shanghai, People's Republic of China, and has served as an assistant engineer with the No. I Bureau of Rail-roads and as an instructor in the Department of Materials Engineering at the Shanghai Institute of Building Materials.
David Darwin, FACI, Deane E. Ackers Professor of Civil Engineering and Di-rector of the Structural Engineering and Materials Laboratory at the Univer-sity of Kansas. He is a member of the Board of Direction and the Technical Activities Committee and is Past President of the Kansas Chapter of ACI. He is also a member and past-chairman of ACI Committee 224, Cracking. He is a member of ACI Committee 408, Bond and Development of Reinforcement; ACI-ASCE Committee 445, Shear and Torsion; ACI Committee 446, Fracture Mechanics; ACI-ASCE Committee 447, Finite Element Analysis of Reinforced Concrete Structures; and the Concrete Materials Research Council.
elasticity E;, and the initial Poisson's ratio "; Material response is compared based on strain rate , water-ce-ment ratio (wlc), and sand-cement ratio (sic). Details of this study are provided in Reference 24.
RESEARCH SIGNIFICANCE This experimental study investigates the strain-rate-
sensitive behavior of saturated cement paste and mor-tar in compression. The stress-strain response of these materials is found to be significantly sensitive to the strain rate. The results indicate that the peak stress will increase with each order of magnitude increase in strain rate. The strain at peak stress first decreases, then in-creases with an increase in strain rate. The results clearly show that the initial elastic moduli of the mate-rials also increase significantly with each order of mag-nitude increase in strain rate, which emphasizes how very few aspects of the response of these materials in compression can be considered independent of strain rate. This study has added significance because strain-rate tests are most often run on partially dried speci-mens (a complete lack of moisture control is not un-common) and data from tests conducted under fully saturated conditions, as described in this paper, are sparse.
EXPERIMENTAL PROGRAM Materials
Cement - Type I portland cement with the follow-ing composition was used: tricalcium silicate = 51.1 percent, dicalcium silicate = 22.3 percent, tetracalcium aluminoferrite = 9.5 percent, and tricalcium aluminate = 7 percent.
Fine aggregate - The fine aggregate was river sand consisting mainly of quartz, with 10 to 15 percent feld-spar. Larger particles contained some limestone and dolomite. Fineness modulus = 2.91, bulk specific gravity (saturated surface dry) = 2.61, absorption = 0.79 percent. Source: Kansas River, Lawrence, Kansa8. The sand was passed through a No. 4 sieve before use.
Mix proportions - Three water-cement ratios (wlc), 0.3, 0.4, and 0.5, were used for cement paste.and mor-tar. Concrete mixtures were proportioned for each w I c
ACI Materials Journal I September-October 1990
Bottom Platen~ ~1"
Fig. 1 - Schematic of test setup
to obtain the sand-cement ratio (sic) for the corre-sponding mortar, designated as Mortar A. For wlc = 0.4 and 0.5, a second mortar, Mortar B, was also tested to evaluate the effect of a change in sic upon the re-sponse. Mortar A with wlc = 0.3 had a sic of 0.97. For wlc = 0.4, Mortar A had a sic of 1.59, and Mor-tar B had a sic of 1.97. For wlc = 0.5, Mortar A had a sic of 2.28 and Mortar B had a sic of 1.29.
Test specimens Prismatic test specimens, 1 x 1 x 5 in., were pre-
pared using steel molds. The constituents were mixed according to ASTM C 305-87, 2' except that the sand was oven-dried at 105 C for 24 hr and then presoaked for 5 min before mixing. The specimens were cast in a vertical position. The molds were filled in three equal layers. The degree of consolidation was adjusted to ac-count for the stiffness of the plastic material. For wlc = 0.5, each layer was hand-rodded 25 times using a V-i-in. diameter steel rod. For wlc = 0.3 and 0.4, the molds were bolted to a vibrating table with a frequency of 60 cycles/sec and an amplitude of 0.006 in. Each layer was vibrated for 2.5 min for wlc = 0.3 and 2 min for wlc = 0.4. The molds were sealed at the top.
During the first 24 hr, the molds were stored in a horizontal position to reduce the effects of bleeding. The specimens were then removed from the molds and stored in lime-saturated water until the time of test.
Prior to te